Solid-State Syntheses of Coordination Polymers by Thermal Conversion of Molecular Building Blocks and Polymeric Precursors
Daniel Lässig; Jörg Lincke; Renata Gerhardt; Harald Krautscheid; Inorganic Chemistry 51 (2012) 6180–6189; doi:10.1021/ic300235s

data_4329339
_publ_contact_author_address
;
Universit\"at Leipzig
Fakult\"at f\"ur Chemie und Mineralogie
Institut f\"ur Anorganische  Chemie
Johannisallee 29
D-04103 Leipzig
Germany
;
_publ_contact_author_email       Krautscheid@rz.uni-leipzig.de
_publ_contact_author_fax         00493419736199
_publ_contact_author_name
;
Harald Krautscheid
;
_publ_contact_author_phone       00493419736172
_publ_section_title
;
 Solid-State Syntheses of Coordination Polymers by Thermal Conversion of
 Molecular Building Blocks and Polymeric Precursors
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              6180
_journal_page_last               6189
_journal_paper_doi               10.1021/ic300235s
_journal_volume                  51
_journal_year                    2012
_chemical_formula_moiety         'C10 H9 N3 O2'
_chemical_formula_sum            'C10 H9 N3 O2'
_chemical_formula_weight         203.20
_chemical_name_systematic
;
4-(3-methyl-4H-1,2,4-triazol-4-yl)benzoic acid
;
_space_group_IT_number           61
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      61
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            16
_cell_length_a                   10.6417(8)
_cell_length_b                   21.0934(19)
_cell_length_c                   17.095(2)
_cell_measurement_reflns_used    7940
_cell_measurement_temperature    213(2)
_cell_measurement_theta_max      25.00
_cell_measurement_theta_min      1.65
_cell_volume                     3837.3(6)
_computing_cell_refinement       'STOE X-AREA'
_computing_data_collection       'STOE X-AREA'
_computing_data_reduction        'STOE X-AREA, STOE X-RED'
_computing_molecular_graphics    'DIAMOND 3.2'
_computing_publication_material  'WinGX publication routines (Farrugia, 1999)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      213(2)
_diffrn_detector_area_resol_mean 6.67
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'STOE IPDS-I'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0816
_diffrn_reflns_av_sigmaI/netI    0.0513
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            16159
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.15
_diffrn_standards_number         none
_exptl_absorpt_coefficient_mu    0.102
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.407
_exptl_crystal_description       prism
_exptl_crystal_F_000             1696
_exptl_crystal_size_max          0.50
_exptl_crystal_size_mid          0.23
_exptl_crystal_size_min          0.10
_refine_diff_density_max         0.198
_refine_diff_density_min         -0.185
_refine_diff_density_rms         0.040
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.887
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     275
_refine_ls_number_reflns         3374
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.887
_refine_ls_R_factor_all          0.0576
_refine_ls_R_factor_gt           0.0377
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0530P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0889
_refine_ls_wR_factor_ref         0.0937
_reflns_number_gt                2339
_reflns_number_total             3374
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic300235s_si_002_2.cif
_cod_data_source_block           H(H-Me-trz-pba)_II
_cod_original_cell_volume        3837.3(7)
_cod_database_code               4329339